| ||Format||Pages||Price|| |
|9||$50.00||  ADD TO CART|
|Hardcopy (shipping and handling)||9||$50.00||  ADD TO CART|
Significance and Use
5.1 This practice is intended primarily for the automated or semi-automated ultrasonic examination of butt fusion joints used in the construction of polyethylene piping systems.
5.2 Polyethylene piping has been used in lieu of steel alloys in the petrochemical, power, water, gas distribution and mining industries due to its reliability and resistance to corrosion and erosion. Recently, polyethylene pipe has also been used for nuclear safety-related cooling water applications.
5.3 Two ultrasonic techniques have proven useful to provide examination of fusion joint integrity; Ultrasonic time-of-flight-diffraction (TOFD) and phased array ultrasonic testing (PAUT). These techniques are often considered complementary but may be used independently of each other. The choice of the technique used may depend on a variety of parameters including diameter, thickness, surface access, detection capabilities near surfaces, and quality level required.
5.4 The joining process can be subject to a variety of flaws including, but not limited to: lack of fusion, particulate contamination, inclusions, and voids.
5.5 Polyethylene material can have a range of acoustic characteristics that make butt joint examination difficult. Acoustic velocity of the material is similar to that commonly used for ultrasound wedge materials, making it difficult to use these materials to achieve appropriate refraction of sound at the interface. Polyethylene materials are highly attenuative, which often limits the use of higher ultrasonic frequencies. It also exhibits a natural high frequency filtering effect. An example of the range of acoustic characteristics is provided in . The table notes the wide range of acoustic velocities reported in the literature. This makes it essential that the reference blocks are made of the same cell classification as that examined. This shall be confirmed by measuring the acoustic velocity of the pipe being examined. When using PAUT as the examination technique, the acoustic velocity of the reference block shall be within ±50 m/s of the examined pipe material being examined.
5.6 Polyethylene is reported to have a shear velocity of 987 m/s. However, due to extremely high attenuation in shear mode (on the order of 5 dB/mm (127 dB/inch) at 2 MHz) no practical examinations are carried out using shear mode (. )
5.7 Due to the wide range of applications, joint acceptance criteria for polyethylene pipe are usually project-specific.
5.8 A typical butt fusion joint in polyethylene pipe has a pronounced bead profile similar to that illustrated in where the bead is shown on the outer and inner surface of the pipe.
5.9 TOFD, when used on polyethylene, is simplified in that mode-converted signals are virtually eliminated due to the high attenuation of the shear mode. However, the near surface and far surface dead zones associated with TOFD may be considered limitations if determined to be excessive for the detection requirements.
5.10 PAUT can be used to address the near surface dead zone that occurs with TOFD.
1.1 This standard practice establishes procedures for ultrasonic testing (UT) of butt fusion joints in polyethylene pipe. Although high density polyethylene (HDPE) and medium density polyethylene (MDPE) materials are most commonly used, the procedures described may apply to other types of polyethylene.
Note 1: The notes in this specification are for information only and shall not be considered part of this specification.
Note 2: This standard references HDPE and MDPE for pipe applications as defined by Specification .
1.2 This standard practice does not address ultrasonic examination of electrofusion joints (coupling joints), socket joints, or saddles.
1.3 This practice provides two ultrasonic examination procedures. Each has its own merits and requirements for examination and shall be selected as agreed upon in a contractual document.
1.3.1 Examination Procedure A, Time of Flight Diffraction (TOFD), uses a pair of probes, one transmitting and the other receiving. The procedure requires access to both sides of the joint from one surface. Provided that position encoding is used, the procedure can be conducted by semi-automated or automated means that provide recoded imaging.
1.3.2 Examination Procedure B, Phased Array Ultrasonic Testing (PAUT), uses low velocity refracting wedges or water gaps to produce angled compression mode pulses. The procedure can be applied where access is limited to one side of the joint from one surface. Provided that position encoding is used, the procedure can be conducted by semi-automated or automated means that provide recoded imaging.
1.4 The practice is intended to be used on thicknesses of 9 to 60 mm (0.375 to 2.4 in.) and diameters 100 mm (4 in.) and greater. Greater and lesser thicknesses and lesser diameters may be tested using this standard practice if the technique can be demonstrated to provide adequate detection on mockups of the same wall thickness and geometry.
1.5 This practice does not specify acceptance criteria.
1.6 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D3350 Specification for Polyethylene Plastics Pipe and Fittings Materials
E494 Practice for Measuring Ultrasonic Velocity in Materials
E543 Specification for Agencies Performing Nondestructive Testing
E1316 Terminology for Nondestructive Examinations
E2373 Practice for Use of the Ultrasonic Time of Flight Diffraction (TOFD) Technique
E2700 Practice for Contact Ultrasonic Testing of Welds Using Phased Arrays
F2620 Practice for Heat Fusion Joining of Polyethylene Pipe and Fittings
Aerospace Industries Association DocumentNAS 410 Certification and Qualification of Nondestructive Testing Personnel Available from Aerospace Industries Association (AIA), 1000 Wilson Blvd., Suite 1700, Arlington, VA 22209, http://www.aia-aerospace.org.
ISO StandardISO 9712 Non-Destructive TestingQualification and Certification of NDT Personnel Available from International Organization for Standardization (ISO), ISO Central Secretariat, BIBC II, Chemin de Blandonnet 8, CP 401, 1214 Vernier, Geneva, Switzerland, http://www.iso.org.
ICS Number Code 25.160.40 (Welding joints and welds)
UNSPSC Code 13102017(High Density Polyethylene HDPE); 13102019(Medium Density Polyethylene MDPE); 40170000(Pipe piping and pipe fittings)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E3044 / E3044M-16e1, Standard Practice for Ultrasonic Testing of Polyethylene Butt Fusion Joints, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top